Amorphous Materials: A Structural Perspective
Amorphous workshop PPXRD-11
Simon Bates: Triclinic Labs
This document was presented at PPXRD -Pharmaceutical Powder X-ray Diffraction Symposium
Sponsored by The International Centre for Diffraction Data
This presentation is provided by the International Centre for Diffraction Data in cooperation with the authors and presenters of the PPXRD symposia for the express purpose of educating the scientific community.
All copyrights for the presentation are retained by the original authors.
The ICDD has received permission from the authors to post this material on our website and make the material available for viewing. Usage is restricted for the purposes of education and scientific research.
ICDD Website - www.icdd.comPPXRD Website www.icdd.com/ppxrd
Where to begin our study of structure in the amorphous state?
A good place to start is to reference known boundaries to the definition of structure.
Ideal Crystalline: A solid with long-range order (periodic or aperiodic) any solid having an essentially discrete diffraction diagram IUCr 1992
Ideal Non-crystalline: A liquid (or solid) possessing no long-range order. any sample having an essentially continuous diffraction diagram
The ideal solid crystal and ideal liquid non-crystal give two equilibrium thermodynamic reference points.
Crystalline and non-crystalline diffraction
Discrete X-ray powder pattern for: Fructose.
Continuous X-ray powder pattern for: Water.
Crystalline: any solid having an essentially discrete diffraction diagram IUCr 1992
What is X-ray amorphous X-ray amorphous powder patterns are continuous in nature (non-crystalline) indicating that the sample has no long-range order and is macroscopically isotropic in nature. However, the X-ray amorphous pattern is a finger print of the short-range order.
RCN: Random Connected Network (disordered crystal). - Local Order retains
crystalline symmetry - Distances and orientations
follow a Random Walk type disorder
RCP: Random Close Packing (frozen liquid) - Random Close Packing
driven by short range interactions (VdW)
- Local order related to molecular shape
Kinetically modified liquid: High T model
Kinetically modified crystal: Low T model
Kinetic Glassy material
Is the concept of structure even important for kinetic glassy material?
Glass transition, Tg, viscosity ~ 10^13 Poise (~10^12 Pa.s) Giulio Biroli: Seminaire Poincare XIII (2009) 37 - 67
Angell plot for super-cooled liquids scaled to glass transition temperature (Tg) shows the different behavior for strong and fragile glasses. Difference in behavior is thought to be related to differences in structural cooperativity. Strong glasses have the same local structure above and below Tg with viscosity related to bond breaking. Scales with the number of bonds. Fragile glasses rapidly lose their local structure below Tg. Non linear viscosity change is related to the growth of cooperative local structure approaching Tg. Scales with length scale of cooperative order.
What is structure in super-cooled liquids?
Molecules exert a long range attractive force on each other
At short distances, molecules repel each other
Thermal motion tends to push molecules further apart at high temperatures
Cooling allows molecules to pack more closely and act more cooperatively
At low temperatures, short range repulsion drives local ordering
gasses liquids super-cooled liquids represent a continuum of isotropic systems with no long-range order.
Can we say anything about long-range order in super-cooled liquids
Spatially, a super-cooled liquid can be considered to be a mosaic of locally ordered regions (each of which represents a local energy minima) isolated from each other by high energy barriers
Configurational Entropy Sc ~ log(Nf)/Nf Nf ~ number of different free energy states available.
Experimental determination of local order will average over the huge number of local states
What does X-ray Powder Diffraction measure for a super-cooled liquid?
Coherent X-ray diffraction from each local packing minima will contribute an individual XRPD profile. Each individual profile is incoherently averaged to give a single mean coherent XRPD response for the sample. The mean response essentially represents the average local order in the sample.
1 2 3 4
Laboratory XRPD averages spatially and over the duration of the measurement insensitive to Tg
In addition to averaging, what other limitations are introduced by the XRPD measurement?
Half cone angle:: gamma From self avoiding random walk Cos(gamma) = (1/(N^(1-x)) Where N is number of units and (x) typically lies between 0.5 and 0.8
Scherrer equation Peak_broadening ~ K /(N d cos(2)) (peak broadening in radians)
Consider random close packing as a self-avoiding random walk
Evolution of gamma gives effective size limit to coherently diffracting clusters for XRPD: Probability of finding a unit in the correct place.
coherent limit ~ N d Where N = number of units and d is size of packing unit
XRPD from a randomly close packed material will have a universal form where peak width is only a function of its position
N=5 ~9.8% strain
So XRPD patterns collected on randomly close packed systems will all look the same?
The universal nature of XRPD patterns from random systems is only with respect to the peak width as a function of peak position. The actual peak position and peak area will be unique to the system of interest!
Crystalline materials also have a universal peak width determined by the instrument alone. For crystalline materials, peak broadening is related to micro-structure. Random materials also have a universal peak width where peak sharpening is related to micro-structure.
Change processing conditions
Random walk N = 5
Random walk N = 5
Are amorphous forms that exhibit different micro-structure and stabilities polyamorphic?
Traditionally, changes in micro-structure are not consider to be new structural polymorphs. The crystal structure is the thermodynamic state and any micro-structure is a
kinetic modification. A kinetically modified crystal form can exhibit different physical and chemical
properties like solubility but is not a new polymorph.
For a glassy material, the super-cooled liquid is the underlying thermodynamic state. Different glassy states with differing micro-structure and configurational
entropy can be considered to be kinetic modifications and may exhibit different physical and chemical properties.
One liquid form == One glassy form. Water is believed to have 2 thermodynamic liquid forms and therefore can
exhibit 2 glassy polymorphs.
But water has more than 2 amorphous forms?
Proposed critical point for low density and high density water
Water has many solid forms and at least 3 different X-ray amorphous forms: low density LDA, high density HDA, and very high density VHDA. LDA and HDA are considered to be glassy forms related to the proposed different low and high density water forms. VHDA is proposed to be a crushed crystal form and often not considered to be a glass.
Including non-equilibrium events into the phase diagram of water introduces a new state of water - Amorphous Ice. Although difficult to make on earth. Amorphous ice is most likely the most common form of water in space.
Rapid quench > 10^5 K/s
X-ray amorphous forms include any material where the mean structural coherence length is or the order of 5 basic units (e.g. atoms, molecules, unit cells). Includes: Liquids, Glasses, crushed Crystals (sometimes), Meso-phases (sometimes) and potentially very small Nano-crystals. Rapid compression
So how do we figure out which type of amorphous short range order we have?
The first step is to measure an appropriate XRPD pattern of the sample of interest.
Background at low angles background at high angles.
You can use a larger step size 0.08 1.2 degrees 2Theta (Cu Kalpha)
Most important is to increase count time (> 4 10 seconds per point)
Next step is to isolate the Total Diffraction Response from the sample by removing a calibrated instrumental background and binning the data to maximize information content per point.
When performing detailed PDF modeling, the background may need to be refined during the modeling.
At this point, we can perform either direct analysis of the data or indirect analysis via a molecular model.
Examples of measured data for liquid water and data pre-processing
Typically, a measurement range of 2.0 80 degrees 2Theta is used (Cu Kalpha). For more accurate PDF type work, measurements to higher angles may be needed. Data collected at higher angles require longer count times.
Data binning removes data points leaving only those required to define the XRPD pattern. Maximize information content per data point.
Total diffraction response
Direct Analysis based upon universal random material halo shape